Simulation of crack propagation in alumina with ab-initio based polarizable force field Stephen Hocker,1 Philipp Beck,2 Siegfried Schmauder,1 Johannes Roth,2 and Hans-Rainer Trebin2 1)

Institut f¨ ur Materialpr¨ ufung, Werkstoffkunde und Festigkeitslehre (IMWF), Universit¨ at Stuttgart, Pfaffenwaldring 32, 70550 Stuttgart, Germany 2) Institut f¨ ur Theoretische und Angewandte Physik (ITAP), Universit¨ at Stuttgart, Pfaffenwaldring 57, 70550 Stuttgart, Germany

arXiv:1112.0563v4 [cond-mat.mtrl-sci] 29 Feb 2012

(Dated: 1 March 2012)

We present an effective atomic interaction potential for crystalline α-Al2 O3 generated by the program potfit. The Wolf direct, pairwise summation method with spherical truncation is used for electrostatic interactions. The polarizability of oxygen atoms is included by use of the Tangney-Scandolo interatomic force field approach. The potential is optimized to reproduce the forces, energies and stresses in relaxed and strained configurations as well as {0001}, {10¯ 10} and {11¯ 20} surfaces of Al2 O3 . Details of the force field generation are given, and its validation is demonstrated. We apply the developed potential to investigate crack propagation in α-Al2 O3 single crystals. I.

INTRODUCTION

Aluminum oxide is the most commonly used ceramic in technological applications. Due to its insulating properties, it is frequently adopted in microelectronic devices, i.e., field effect transistors, integrated circuits or superconducting quantum interference devices. Another important field of application is the coating of metallic components. Alumina covering aluminum is known to prevent further oxidation of the metal. Since alumina is characterized by a high melting point and also a high degree of hardness, applications at high temperatures and high mechanical demands are possible. Mechanical properties such as tensile strengths and fracture processes are of high importance regarding these applications. Because surfaces and internal interfaces play an important part in these technologies, numerical modelling is often focused on such systems. Due to this technological significance, alumina and metal/alumina interfaces were frequently investigated experimentally1–3 and by ab-initio methods.4–7 Firstprinciples methods are well established for calculating the work of separation or the surface energy. However, the investigation of dynamic processes such as crack propagation requires systems with significantly more atoms and larger timescales than ab-initio based methods nowadays can deal with. Hence, it is an important challenge to develop a suitable interaction force field for classical Molecular Dynamics (MD) simulations. There exist interaction potential approaches for alumina, which reach a good accuracy by using angular dependent terms.8,9 Pair potentials are also widely applied in simulations of alumina10–13 by reason of usually much lower computational demands. Due to the lattice misfit, especially the simulation of interface structures has to be performed with many atoms. Hence, for the simulation of crack propagation, a pair potential is to be favored concerning the computational effort. Many-body effects can be important for correctly describing bond angles and bond-bending vibration fre-

quencies in oxides. However, for SiO2 14–16 and MgO,16 it was shown that an accurate description can be achieved without angular dependent terms, but with polarizable oxygen atoms. There, the potential model of Tangney and Scandolo14 (TS) is applied, in which the dipole moments of oxygen atoms are determined self-consistently from the local electric field of surrounding charges and dipoles. In Ref. 16, the computational effort in simulations scales linearly in the number of particles, which is due to the Wolf summation.17 We apply this combination of the TS model and the Wolf summation method in the potential generation as well as in simulations. An effective atomic interaction potential is generated with the program potfit .18 The potential parameters are optimized by matching the resulting forces, energies and stresses with respective ab-initio values with the force matching method.19 Simulations are performed with the MD code IMD.20 A detailed description of the adopted methods and the potential generation is given in Sec. II. MD simulations and ab-initio calculations which were performed in order to validate the obtained force field are presented in Sec. III. As a first appplication of the new potential, we investigate crack propagation of alumina single crystals. To our knowledge, these are the first MD simulations of crack propagation in alumina with a potential that takes into account the polarizability of oxygen atoms. Results of these simulations are shown in IV. Finally, conclusions and an outlook are presented in Sec. V.

II.

FORCE FIELD GENERATION

A.

Tangney-Scandolo force field

The TS force field is a sum of two contributions: a short-range pair potential of Morse-Stretch (MS) form, and a long-range part, which describes the electrostatic interactions between charges and induced dipoles on the

2 oxygen atoms. The MS interaction between an atom of type i and an atom of type j has the form " # r γ r ij ij ij UijMS = Dij exp[γij (1 − 0 )] − 2 exp[ (1 − 0 )] , rij 2 rij (1) with rij = |rij |, rij = rj − ri and the model parameters 0 Dij , γij and rij , which have to be determined during the force field generation. Because the dipole moments depend on the local electric field of the surrounding charges and dipoles, a selfconsistent iterative solution has to be found. In the TS approach, a dipole moment pni at position ri in iteration step n consists of an induced part due to an electric field E(ri ) and a short-range part pSR due to the short-range i interactions between charges qi and qj . Following Rowley et al.,21 this contribution is given by pSR = αi i

X qj rij j6=i

3 rij

fij (rij )

(2)

is decomposed into two terms Erqq and Ekqq by inserting a unity of the form 1 = erfc(κr) + erf(κr) with the error function 2 erf(κr) := √ π

(8)

0

The splitting parameter κ controls the distribution of energy between the two terms. The short-ranged erfc term is summed up directly, while the smooth erf term is Fourier transformed and evaluated in reciprocal space. This restricts the technique to periodic systems. However, the main disadvantage is the scaling of the computational effort with the number of particles in the simulation box, which increases as O(N 3/2 ),22 even for the optimal choice of κ. Wolf et al.17 designed a method with linear scaling properties O(N ) for Coulomb interactions. By taking into account the physical properties of the system, the reciprocal-space term Ekqq is disregarded. It can be written as

with

2

fij (rij ) = cij

4 X (bij rij )k

k=0

k!

Ekqq e

−bij rij

.

pni = αi E(ri ; {pjn−1 }j=1,N , {rj }j=1,N ) + pSR i ,

(4)

where αi is the polarizability of atom i and E(ri ) the electric field at position ri , which is determined by the dipole moments pj in the previous iteration step. Taking into account the interactions between charges U qq , between dipole moments U pp and between a charge and a dipole U pq , the total electrostatic contribution is given by U EL = U qq + U pq + U pp ,

(5)

and the total interaction is U tot = U MS + U EL .

(6)

Wolf summation

The electrostatic energies of a condensed system are described by functions with r−n dependence, n ∈ {1, 2, 3}. For point charges (r−1 ) it is common to apply the Ewald method, where the total Coulomb energy of a set of N ions, E qq

(9)

where S(k) is the charge structure factor and V the volume of the simulation box. The charge structure factor is the Fourier transform of the charge-charge autocorrelation function. In condensed matter, the charges screen each other; the approach yields proper results in liquids and largely also in solids. This means that for small magnitudes of the wave vectors k, the charge structure factor is also small. In previous studies16,23 it was shown that the reciprocal-space term is indeed negligible compared to the real-space part, provided that the splitting parameter κ is chosen small enough. As however a smaller κ results in a larger real-space cutoff rc , the latter has to be chosen three or four times the size of a typical shortrange cutoff radius in metals. In a recent study16 a cutoff radius of only 8 ˚ A was sufficient to describe the electrostatics of liquid silica and magnesia accurately. In addition, a continuous and smooth cutoff of ˜ qq (rij ) = the remaining screened Coulomb potential E −1 qi qj erfc(κrij )rij is adopted at rc by shifting the potential so that it goes to zero smoothly in the first two derivatives at r = rc . We use the Wolf method for Coulomb and dipolar interactions. For more information about the Wolf summation of dipole contributions, the estimation of errors attended by this method and a detailed analysis of the energy conservation in MD simulations see Ref. 23. C.

N

exp(− |k| 2π X 4κ2 ) = , S(k) V |k|2 k6=0 |k|

Institut f¨ ur Materialpr¨ ufung, Werkstoffkunde und Festigkeitslehre (IMWF), Universit¨ at Stuttgart, Pfaffenwaldring 32, 70550 Stuttgart, Germany 2) Institut f¨ ur Theoretische und Angewandte Physik (ITAP), Universit¨ at Stuttgart, Pfaffenwaldring 57, 70550 Stuttgart, Germany

arXiv:1112.0563v4 [cond-mat.mtrl-sci] 29 Feb 2012

(Dated: 1 March 2012)

We present an effective atomic interaction potential for crystalline α-Al2 O3 generated by the program potfit. The Wolf direct, pairwise summation method with spherical truncation is used for electrostatic interactions. The polarizability of oxygen atoms is included by use of the Tangney-Scandolo interatomic force field approach. The potential is optimized to reproduce the forces, energies and stresses in relaxed and strained configurations as well as {0001}, {10¯ 10} and {11¯ 20} surfaces of Al2 O3 . Details of the force field generation are given, and its validation is demonstrated. We apply the developed potential to investigate crack propagation in α-Al2 O3 single crystals. I.

INTRODUCTION

Aluminum oxide is the most commonly used ceramic in technological applications. Due to its insulating properties, it is frequently adopted in microelectronic devices, i.e., field effect transistors, integrated circuits or superconducting quantum interference devices. Another important field of application is the coating of metallic components. Alumina covering aluminum is known to prevent further oxidation of the metal. Since alumina is characterized by a high melting point and also a high degree of hardness, applications at high temperatures and high mechanical demands are possible. Mechanical properties such as tensile strengths and fracture processes are of high importance regarding these applications. Because surfaces and internal interfaces play an important part in these technologies, numerical modelling is often focused on such systems. Due to this technological significance, alumina and metal/alumina interfaces were frequently investigated experimentally1–3 and by ab-initio methods.4–7 Firstprinciples methods are well established for calculating the work of separation or the surface energy. However, the investigation of dynamic processes such as crack propagation requires systems with significantly more atoms and larger timescales than ab-initio based methods nowadays can deal with. Hence, it is an important challenge to develop a suitable interaction force field for classical Molecular Dynamics (MD) simulations. There exist interaction potential approaches for alumina, which reach a good accuracy by using angular dependent terms.8,9 Pair potentials are also widely applied in simulations of alumina10–13 by reason of usually much lower computational demands. Due to the lattice misfit, especially the simulation of interface structures has to be performed with many atoms. Hence, for the simulation of crack propagation, a pair potential is to be favored concerning the computational effort. Many-body effects can be important for correctly describing bond angles and bond-bending vibration fre-

quencies in oxides. However, for SiO2 14–16 and MgO,16 it was shown that an accurate description can be achieved without angular dependent terms, but with polarizable oxygen atoms. There, the potential model of Tangney and Scandolo14 (TS) is applied, in which the dipole moments of oxygen atoms are determined self-consistently from the local electric field of surrounding charges and dipoles. In Ref. 16, the computational effort in simulations scales linearly in the number of particles, which is due to the Wolf summation.17 We apply this combination of the TS model and the Wolf summation method in the potential generation as well as in simulations. An effective atomic interaction potential is generated with the program potfit .18 The potential parameters are optimized by matching the resulting forces, energies and stresses with respective ab-initio values with the force matching method.19 Simulations are performed with the MD code IMD.20 A detailed description of the adopted methods and the potential generation is given in Sec. II. MD simulations and ab-initio calculations which were performed in order to validate the obtained force field are presented in Sec. III. As a first appplication of the new potential, we investigate crack propagation of alumina single crystals. To our knowledge, these are the first MD simulations of crack propagation in alumina with a potential that takes into account the polarizability of oxygen atoms. Results of these simulations are shown in IV. Finally, conclusions and an outlook are presented in Sec. V.

II.

FORCE FIELD GENERATION

A.

Tangney-Scandolo force field

The TS force field is a sum of two contributions: a short-range pair potential of Morse-Stretch (MS) form, and a long-range part, which describes the electrostatic interactions between charges and induced dipoles on the

2 oxygen atoms. The MS interaction between an atom of type i and an atom of type j has the form " # r γ r ij ij ij UijMS = Dij exp[γij (1 − 0 )] − 2 exp[ (1 − 0 )] , rij 2 rij (1) with rij = |rij |, rij = rj − ri and the model parameters 0 Dij , γij and rij , which have to be determined during the force field generation. Because the dipole moments depend on the local electric field of the surrounding charges and dipoles, a selfconsistent iterative solution has to be found. In the TS approach, a dipole moment pni at position ri in iteration step n consists of an induced part due to an electric field E(ri ) and a short-range part pSR due to the short-range i interactions between charges qi and qj . Following Rowley et al.,21 this contribution is given by pSR = αi i

X qj rij j6=i

3 rij

fij (rij )

(2)

is decomposed into two terms Erqq and Ekqq by inserting a unity of the form 1 = erfc(κr) + erf(κr) with the error function 2 erf(κr) := √ π

(8)

0

The splitting parameter κ controls the distribution of energy between the two terms. The short-ranged erfc term is summed up directly, while the smooth erf term is Fourier transformed and evaluated in reciprocal space. This restricts the technique to periodic systems. However, the main disadvantage is the scaling of the computational effort with the number of particles in the simulation box, which increases as O(N 3/2 ),22 even for the optimal choice of κ. Wolf et al.17 designed a method with linear scaling properties O(N ) for Coulomb interactions. By taking into account the physical properties of the system, the reciprocal-space term Ekqq is disregarded. It can be written as

with

2

fij (rij ) = cij

4 X (bij rij )k

k=0

k!

Ekqq e

−bij rij

.

pni = αi E(ri ; {pjn−1 }j=1,N , {rj }j=1,N ) + pSR i ,

(4)

where αi is the polarizability of atom i and E(ri ) the electric field at position ri , which is determined by the dipole moments pj in the previous iteration step. Taking into account the interactions between charges U qq , between dipole moments U pp and between a charge and a dipole U pq , the total electrostatic contribution is given by U EL = U qq + U pq + U pp ,

(5)

and the total interaction is U tot = U MS + U EL .

(6)

Wolf summation

The electrostatic energies of a condensed system are described by functions with r−n dependence, n ∈ {1, 2, 3}. For point charges (r−1 ) it is common to apply the Ewald method, where the total Coulomb energy of a set of N ions, E qq

(9)

where S(k) is the charge structure factor and V the volume of the simulation box. The charge structure factor is the Fourier transform of the charge-charge autocorrelation function. In condensed matter, the charges screen each other; the approach yields proper results in liquids and largely also in solids. This means that for small magnitudes of the wave vectors k, the charge structure factor is also small. In previous studies16,23 it was shown that the reciprocal-space term is indeed negligible compared to the real-space part, provided that the splitting parameter κ is chosen small enough. As however a smaller κ results in a larger real-space cutoff rc , the latter has to be chosen three or four times the size of a typical shortrange cutoff radius in metals. In a recent study16 a cutoff radius of only 8 ˚ A was sufficient to describe the electrostatics of liquid silica and magnesia accurately. In addition, a continuous and smooth cutoff of ˜ qq (rij ) = the remaining screened Coulomb potential E −1 qi qj erfc(κrij )rij is adopted at rc by shifting the potential so that it goes to zero smoothly in the first two derivatives at r = rc . We use the Wolf method for Coulomb and dipolar interactions. For more information about the Wolf summation of dipole contributions, the estimation of errors attended by this method and a detailed analysis of the energy conservation in MD simulations see Ref. 23. C.

N

exp(− |k| 2π X 4κ2 ) = , S(k) V |k|2 k6=0 |k|